## Design of a Low Cost Single Gate Planar Junctionless Transistor over

## FD-SOI Wafer

### Arian Nowbahari

### Relatore Matteo Cocuzza

### Supervisore Luca Marchetti

### Final Project Report for the Master in Electronic Engineering

### Department of Electronics and Telecommunications Polytechnic University of Turin

### Department of Microsystems

### University of South-Eastern Norway

### Junctionless Transistor over FD-SOI Wafer

### Arian Nowbahari Supervised by:

### Matteo Cocuzza Luca Marchetti

## Abstract

Owing to the simple and cost-effective fabrication process and enhanced performance
with respect to conventional MOSFETs, junctionless transistors are becoming a sig-
nificant topic of research. In fact they are characterized by the absence of any pn
junctions in their physical structure, thus avoiding one of the most expensive and
difficult step in transistor fabrication, that is the implantation of source and drain
contacts. After the fabrication of the first junctionless transistors (nanowire) in
2010, many others were proposed such as junctionless FinFETs, GAAFETs, double
gate, and planar. The critical point is that these devices, even if easier to fabricate
with respect to conventional transistors, are anyway very expensive, thus restricting
the possibility to realize prototypes in research and industrial field. For this reason
a low cost planar junctionless transistor is proposed. First the design of its struc-
ture is carried out, by sizing and deciding its physical components on the basis of
parametric computations and analytical models; the designed transistor has a chan-
nel length of 500nm, a device layer thickness of 600nm, a low doping concentration
(1e15cm^{−3}), and is characterized by an operating range of 1V. The metallization
material is aluminum. Next a low cost fabrication process that does not require
any implantation step is proposed and discussed in detail, considering also source
of non-idealities. Then the simulations results obtained through COMSOL Multi-
physics are reported, confirming the expected principle of operation of the designed
transistor. At the end two papers written for this master thesis are attached. The
first one is a paper review that provides a classification and critical analysis in terms
of performance engineering of the various junctionless transistors. It was decided to
write such state of the art because most of the reviews about junctionless transistors
were written in 2010-2013, thus not containing the last developments. The second
one is a journal article in which a method for the extraction from CAD software
of one of the most important parameters in junctionless transistors, that is the de-
pletion width extension, is proposed. The algorithm fit the analytical model, and
allows to quantitatively distinguish the carrier concentration at the depletion region
boundary.

I would first like to thank my main supervisor Prof.Cocuzza of the Department of Applied Science and Technology at the Polytechnic University of Turin, for giving me the great opportunity of working in a clean room, thus allowing me to put in practice the knowledge required during his lessons.

I would also like to thank my supervisor post doc fellow Luca Marchetti of the De- partment of Microsystems at University of South-Easter Norway for his inestimable guidance during all the project, and for his support in helping me to understand how to write scientific articles. During my six months in Norway I learned a lot from him.

I would also like to acknowledge PhD fellow Avisek Roy of the Department of Mi- crosystems at University of South-Easter Norway for his very valuable comments and suggestions in the analysis of the fabrication process.

I would also like to thank all the master and PhD students, in particular my project colleague Konsam Bishwojit, for the helpful discussions.

Finally, I would like to express my gratitude to my parents for providing me with unfailing support and continuous encouragement throughout my years of study.

Arian Nowbahari

1 Introduction 10

2 Proposed Device 14

2.1 Structure . . . 14

2.2 Operation . . . 15

2.3 Specifications . . . 16

3 Design 18 3.1 Device Layer Thickness . . . 18

3.1.1 Maximum Depletion Width . . . 18

3.1.2 Doping Concentration Estimation . . . 19

3.1.3 Resistivity Measurement . . . 21

3.2 Source and Drain . . . 24

3.2.1 Material Selection . . . 24

3.2.2 Parasitic Resistance Model . . . 27

3.2.3 Aluminum Deposition and Diffusion . . . 33

3.3 Gate . . . 39

3.3.1 Material Selection . . . 39

3.4 Fabrication Process . . . 44

3.4.1 Process Flow . . . 44

3.4.2 Mask . . . 50

3.5 Final Structure . . . 52

4 Simulation 54 4.1 Model definition . . . 54

4.1.1 Structure . . . 54

4.1.2 Parameters . . . 55

4.2 Simulations results . . . 55

4.2.1 Is vs Vg . . . 55

4.2.2 Is vs Vs . . . 61

5 Conclusion 63 A MATLAB Codes 64 A.1 Maximum Depletion Width . . . 64

A.2 Mobility Estimation . . . 65

A.3 Resistivity Measurement . . . 66

A.4 Parasitic resistance analysis . . . 67

A.5 Diffusion Modelling . . . 68

A.6 Flat Band Voltage . . . 69 A.7 Analytical Threshold Voltage . . . 71 A.8 Extracted Threshold Voltage . . . 72

B Papers 74

B.1 Analysis and Classification of Junctionless Transistors: a Paper Review 74 B.2 A Numerical Method to Extract the Depletion Region Width of Pla-

nar Junctionless Transistors . . . 100

1.1 Junctionless transistors literature distribution. . . 12 1.2 Graphical representation of the distribution of the analyzed literature

in the attached paper (Appendix B.1). . . 13 2.1 P-type PJLT Physical Structure. (a) Complete Structure on FDSOI

wafer. (b) Simplified Structure. . . 14 2.2 PJLT principle of operation. (a) Full depletion: no conduction. (b)

Partial depletion: bulk conduction. (c) Accumulation: surface con- duction. . . 15 2.3 Current behavior comparison. (a1) Inversion mode device. (12) Ac-

cumulation mode device. (a3) Junctionless transistor [9]. . . 16 3.1 Maximum Depletion width as a function of the doping concentration. 19 3.2 Flow chart of the algorithm implemented in MATLAB for the mobil-

ity estimation. . . 20 3.3 Graph of the resistivity versus impurity concentration at 300K [14]. . 21 3.4 Schematic of a collinear four probe measurement setup [16]. . . 21 3.5 Probe station used for the resistance measurement in the clean room. 22 3.6 Energy band diagrams of a metal-semiconductor (p-type) junction

with qΦm < qΦ_{s,p}. (a) Before contact. (b) In equilibrium. (c) For-
ward bias. (d) Reverse bias [19]. . . 25
3.7 IV curve for two different doping concentrations [26]. . . 26
3.8 Schematic of the resistance modelling of the junctionless transistor. . 27
3.9 Modelling Rsubas a rectangular box: TSiis the device layer thickness,

d the spacing between the S/D and the gate, W the width of the transistor. . . 27 3.10 Case 1: Fixed W (5µm). Plot of Rsub as a function of the separation

region d, which is ranging from 5µm to 10µm. Wafer under analysis is L (Tab.3.2). . . 28 3.11 Case 1: Fixed d (5µm). Plot of Rsub as a function of the transistor

width W , which is ranging from 5µm to 10µm. Wafer under analysis is L (Tab.3.2). . . 28 3.12 Proposed structure schematic for the reduction of the high parasitic

resistance Rsub (not in scale). . . 29 3.13 More realistic structure schematic for the reduction of the high par-

asitic resistance Rsub (not in scale). . . 29 3.14 Contact resistance of aluminum as a function of doping concentration

for different barrier heights. Solid line (n-type silicon), dotted line (p- type silicon) [31]. . . 30

3.15 Contact resistance of aluminum as a function of resistivity [32]. . . . 31

3.16 Schematic of the junctionless transistor structure after resistance mod- elling (not in scale). . . 31

3.17 Array of contact in a MOSFET [33]. . . 32

3.18 (a)Considering only one contact window. (b) Considering two contact windows. The resistance Rm associated to the metal is not shown. . 32

3.19 Sputter AJA used for testing the aluminum deposition rate in the clean room. . . 33

3.20 Third ellipsometer measurement for the silicon oxide thickness. . . 34

3.21 Wafer used for testing the deposition process after exposure. . . 35

3.22 Wafer used for testing the deposition process after aluminum etching. The dark areas are made of silicon oxide. . . 35

3.23 Concentration profile assuming a temperature of 1300K and a pre- deposited layer of 20nm for different diffusion times. . . 37

3.24 Concentration profile assuming a temperature of 1300K and a pre- deposited layer of 200nm for different diffusion times. . . 38

3.25 Flat band voltage behavior as a function of the doping concentration for an n-type junctionless transistor. . . 40

3.26 Flat band voltage behavior as a function of the doping concentration for an p-type junctionless transistor. . . 41

3.27 Threshold voltage behavior as a function of the doping concentration for an n-type junctionless transistor (tSi = 300nm). . . 42

3.28 Threshold voltage behavior as a function of the doping concentration for an p-type junctionless transistor (tSi = 300nm). . . 42

3.29 Analytical Depletion width of the p-type JLT built on wafer C. The threshold and flat band voltages are indicated. . . 43

3.30 PROC_0: starting point of the proposed fabrication process. . . 44

3.31 PROC_1: wafer covered with PR. The handle substrate is not shown. 44 3.32 PROC_2: wafer after PR exposure and development. . . 45

3.33 PROC_3: DRIE using the PR as mask and the SiO2 as etch stop layer. . . 45

3.34 PROC_4: Wafer after redeposition of PR, exposure, and development. 46 3.35 PROC_5: Aluminum deposition throgh sputtering. . . 46

3.36 PROC_6: after lift off process; corner effects not considered, ideal process. . . 46

3.37 PROC_7: after diffusion process. . . 47

3.38 PROC_8: after deposition and patterning of SiO2. . . 47

3.39 How PROCESS_8 could be affected by mask misalignment. . . 47

3.40 PROC_9: deposition of a thin layer SiO2 (gate oxide). . . 48

3.41 PROC_10: structure after PR development. . . 48

3.42 PROC_11: Structure after aluminum deposition and lift off. . . 48

3.43 PROC_12: Via definition. . . 49

3.44 PROC_12: final structure . . . 49

3.45 MASK_0: transistor separation . . . 50

3.46 MASK_1: p++ regions definition. . . 50

3.47 MASK_2 : gate definition. . . 51

3.48 MASK_3: gate metallization. . . 51

3.49 MASK_4: via definition. . . 51

3.50 MASK_5: source and drain metallization. . . 52

3.51 Proposed single gate planar junctionless transistor; the BOX is not shown (not in scale). . . 52

4.1 P-type PJLT Physical Structure. (a) Complete Structure on FDSOI wafer. (b) Simplified Structure. . . 54

4.2 Implementation in COMSOL Multiphysics of the p-type junctionless transistor. . . 55

4.3 Is vs Vg for a fixed source voltage Vs = 10mV. . . 56

4.4 ELR method: linear extrapolation in the linear region [41]. . . 56

4.5 Application of the ELR method for the threshold voltage extraction.
Solid: Is/V_{g}. Dashed: linear extrapolation of Is/V_{g} at maximum slope. 57
4.6 Solid: transconductance vs gate voltage. Dasehd: vertical line passing
for the minimum. The intercept with the gate voltage axis is at −1.08V . 57
4.7 Solid: source current vs gate voltage. Dashed: linear extrapolation
of Is/V_{g} at maximum slope. . . 58

4.8 Solid: transconductance vs gate voltage. Dashed: linear extrapola-
tion of gm/V_{g} at maximum slope. The x-coordinate of the indicated
star corresponds to the extracted flat band voltage . . . 58

4.9 Hole surface concentration for Vg = 0V. . . 59

4.10 Hole surface concentration for Vg =−0.5V . . . 59

4.11 Hole surface concentration for Vg =−0.75V . . . 60

4.12 Hole surface concentration for Vg =−1V . . . 60

4.13 Hole surface concentration for Vg = 0V and TSi= 300nm. . . 61

4.14 Is/V_{s} for different gate voltages. . . 61

4.15 Is/V_{s} for Vg =−1V . . . 62

4.16 Is/V_{s} for Vg =−2V . . . 62

2.1 Wafers characteristics. . . 17

3.1 Wafers resistances measurement data. . . 22

3.2 Computed wafers resistivities, doping concentrations, and maximum depletion widths. . . 23

3.3 Contact behavior as a function of different materials. . . 25

3.4 Process parameters for aluminum and silicon oxide deposition. . . 34

3.5 Ellipsometer measurement data for the silicon oxide thickness. . . 34

3.6 Profilometer measurement data for the estimation of the photoresist thickness in three different squares. . . 35

3.7 Profilometer measurement data for the estimation of the aluminum thickness in three different squares. . . 36

3.8 Profilometer measurement data for the aluminum thickness. . . 36

3.9 Analytical flat band voltages considering aluminum as gate material and the measured doping concentrations of Tab.3.2. . . 41

3.10 Analytical threshold voltage considering aluminum as gate material and and a gate oxide thickness of 10nm . . . 43

3.11 Geometrical parameters of the designed transistor. . . 52

3.12 Materials of the designed transistors. . . 53

3.13 Doping Concentration, threshold voltage, and flat band voltage of the designed transistor. . . 53

4.1 Parameters used for the COMSOL Multiphysics simulation. . . 55

## Introduction

The concept of junctionless transistor (JLT) was introduced by J.E. Lilienfeld in
1925 [1]. The main characteristic of the Lilienfeld device was the absence of any
pn junction in the physical structure of the transistor. By controlling the voltage
at the gate terminal of this semiconductor device, Lilienfeld was able to deplete the
carriers in a localized region of the substrate. In this manner, it was possible to
control the resistivity of the device and therefore the electrical current through the
transistor. But the technology of that time did not allow him to realize a working
device [2], which required the fabrication of a nanometric substrate layer. Only in
2010 at the Tyndall National Institute, the first junctionless transistor [2] was suc-
cessfully manufactured; J.P. Colinge et al. fabricated a 10nm thick and 1µm long
highly doped (10^{19}cm^{−3}) junctionless nanowire transistor. The device represents
the first one of a new generation of transistors. In fact after its realization, many
others were proposed such as: FinFETs, Gate-All-AroundFETs (GAAFETs), planar
(PJLT), double gate (DGJLT), thin-filmFETs (TFT), and tunnelFETs (TFET). The
advantages of a junction-free structure are numerous such as the absence of doping
concentration gradients [3], which are difficult to precisely control in the nanomet-
ric regime, the absence of junction leakages, simple fabrication process and lower
fabrication cost (since no implantation for source and drain are required) [4]. In
addition, these transistors can provide greater performance with respect to conven-
tional transistors, such as reduced short-channel effects (effective channel length not
reduced by pn junctions) [5] and less degradation of carrier mobility (current flows
in the bulk of the substrate) [6]. For all these reasons it was decided to propose
a design and fabrication of a low cost junctionless transistor. From a fabrication
process point of view, the simplest junctionless transistor is the planar one, which
is usually realized through FDSOI (fully depleted silicon on insulator) technology.

The critical problem is that the clean room available in the facility is a MEMS one.

Therefore this project aims to provide a simple fabrication process, compatible with the available machines in the laboratory, that could lower the fabrication cost of the device. The project is carried out by two master students: one has to find a low cost fabrication method for the realization of SOI wafers, while the other one has to design and simulate the transistor. This thesis, which has as target the design and simulation of the transistor, it structured in two parts: the first one (Sect.3) treats the design of the planar single gate junctionless transistor on the basis of the project specifications and it is divided as it follows:

• design of the device layer thickness on the basis of the doping concentration;

• design of the source and drain contacts, in terms of material and geometry, on the basis of a parasitic resistance model;

• design of the metal gate, by considering influence of the physical parameters on the main electrical quantities;

• step by step fabrication process;

• masks.

The second part (Sect.4), treats the simulation of the device, which is carried out by means of COMSOL Multiphysics, with the aim of:

• verify the designed junctionless transistor in terms of qualitative operation;

• extract the important electrical quantities (e.g. threshold voltage) and com- pare them to the analytical values.

Besides the design and the simulation of the junctionless transistor, two papers for this thesis were written:

1. Analysis and Classification of Junctionless Transistors: a Paper Review;

2. A Numerical Method to Extract the Depletion Region Width of Planar Junc- tionless Transistors.

The first paper is a state of the art of junctionless transistors. The motivation to write a state of the art relies on the fact that most of the paper reviews about this topic were published in 2010-2013, thus not considering the latest developments.

The paper (which is in Appendix B.1) analyzes a total of 118 papers in order to provide a complete overview of the main involved figure of merits. The transistors are classified as it follows:

• Nanowire;

• FinFET;

• Gate-All-Around;

• Planar;

• Thin-Film;

• Double Gate;

• TunnelFET.

And the paper distribution is the one depicted in Fig.1.1.

TFET: 9%

DGJLT: 21%

NW: 19%

TFT: 9%

GAAFET: 12%

FinFET: 18%

PJLT: 11%

TFET:11 DGJLT:25 NW:23 TFT:11 GAAFET:14 FinFET:21 PJLT:13

**Junctionless Transistor Literature Distribution (118 papers)**

Figure 1.1: Junctionless transistors literature distribution.

The graphical representation of the analyzed literature is shown in Fig.1.2 in the next page. The second paper (Appendix B.2) instead was written in order to provide a method to extract the depletion width from CAD software. The motivation to write it relied on the fact that during the simulations it was not possible to precisely define the boundary between the depleted and undepleted part, thus not allowing a qualitative interpretation of the simulations results. By the implementation of the method was possible to verify the limits of the analytical depletion width model.

Moreover the application of the algorithm to different structures demonstrated that the carrier concentration at the boundary of the depletion width is approximately half the doping concentration.

Figure 1.2: Graphical representation of the distribution of the analyzed literature in the attached paper (Appendix B.1).

## Proposed Device

### 2.1 Structure

The proposed device is a planar single gate junctionless transistor over FD-SOI (fully depleted silicon on insulator [7]), depicted in Fig.2.1(a). The main difference with respect to conventional MOSFETs is the absence of any pn junction in the device layer. A planar junctionless transistor (PJLT) realized on FD-SOI is characterized by three layers: a handle substrate (silicon), an insulating layer (BOX, that is buried oxide), and a thin device layer (silicon).

Figure 2.1: P-type PJLT Physical Structure. (a) Complete Structure on FDSOI wafer. (b) Simplified Structure.

As explained in the attached papers (Appendix B), the device layer is typically thin
and highly doped in order to allow a correct device operation. The handle substrate
does not require to be doped unless the designer decides to use it as second gate
terminal or back gate; since the proposed device is a planar single gate junctionless
transistor (PJLT), the simplified structure in Fig.2.1(b) is considered. The device
layer of a PJLT can be uniformly doped if it is highly doped (> 1e19cm^{−3}) and has
a thickness about 10nm [8]: in fact, if the doping concentration is very high and the
film is very thin, the parasitic resistance associated to the regions below the source
and drain contacts is very low. But such thickness is not usually easy to achieve,

since most of the SOI wafers available on the market have a thickness in the range of micrometers. Therefore a possible solution consists into realizing highly doped drain and source wells in order to minimize the parasitic resistances between the channel of the transistor (conductive part of the device layer between the wells) and the source and drain metallizations. In particular, if the device layer is n-doped, then the source and drain wells must be heavily doped with donors (n++). On the other hand, if the device layer is p-doped, then the source and the drain wells must be heavily doped with acceptors (p++). These wells are represented with black regions in Fig.2.1(a).

### 2.2 Operation

A junctionless transistor works differently with respect to inversion mode devices [3].

The principle of operation, which is verified in Sect.4, can be qualitatively described as in Fig.2.2: when the gate voltage is lower than the threshold one, the device layer is fully depleted (Fig.2.2(a)). As the gate voltage is increased to more positive values, electrons are attracted towards the oxide/semiconductor interface, and the depletion region width is reduced, thus a path between the source and the drain below the depletion region is created, and a bulk current is formed (Fig.2.2(b)). If the gate voltage is then increased over the flat band voltage, many electrons are attracted to the semiconductor/oxide interface, thus forming an accumulation layer at the surface (Fig.2.2(c)).

Figure 2.2: PJLT principle of operation. (a) Full depletion: no conduction. (b) Partial depletion: bulk conduction. (c) Accumulation: surface conduction.

As a consequence the positions of the threshold and flat band voltage is very different for inversion mode, accumulation mode, and junctionless transistors (Fig.2.3(a3)).

Figure 2.3: Current behavior comparison. (a1) Inversion mode device. (12) Accu- mulation mode device. (a3) Junctionless transistor [9].

For junctionless transistors the threshold voltage is defined as the gate voltage that fully depletes (OF F state) the device layer (Fig. 2.3(a1)). Thus they are more similar to accumulation mode devices (Fig.2.3(a2)) in terms of threshold voltage definition. Regarding the current, two components can be distinguished: a bulk and an accumulation current. When the gate voltage is greater than the threshold one, partial depletion takes place creating a path in the substrate for the bulk current.

As the gate voltage overcomes the flat band, an accumulation layer is formed at the oxide/semiconductor interface (ON state).

### 2.3 Specifications

The design specifications are the following ones:

• single gate planar junctionless transistor;

• fabrication process compatible with the MEMS clean room;

• photolithographic resolution of maskless machine of 350nm;

• photolithographic resolution of the mask aligner 2µm;

• mask alignment of 100nm (nominal value).

The PJLTs to be designed are going to be fabricated in a MEMS clean room; this implies constraints on the available machines and resolution. For instance no CVD reactors are present, and the only system available for the deposition of materials is a sputtering system. Regarding the photolithography, two machines are present:

a mask aligner mainly used for MEMS devices with a resolution of 2µm, and a maskless machine with a resolution of 350nm. The latter works on the basis of a serial process which is very slow as compared to the MEMS mask aligner. The idea is therefore to use the maskless machine for the critical dimensions, and the mask aligner for the large ones. Regarding the mask alignment, a nominal value of 100nm is provided. Concerning the available wafers, the ones with characteristics in Tab.2.1 are present, and their resistivity is provided in a range ([5-10] Ωcm).

Table 2.1: Wafers characteristics.

Parameter Value

Number 3

Type BSOI

Dopant p-Boron

Resistivity [5-10] Ωcm

Diameter 100mm

Device Layer Thickness 20µm BOX thickness 0.5µm Handle Thickness 380µm

## Design

In this section the proposed design is reported: first the needed device layer thickness is decided, on the basis of the estimated doping concentration; then a parasitic resistance model is analyzed for sizing the geometrical parameters of the device, and finally the fabrication process, together with the masks, is provided.

### 3.1 Device Layer Thickness

### 3.1.1 Maximum Depletion Width

In order to ensure fully depleted SOI technology, i.e. to guarantee that the device layer can be entirely depleted and thus the transistor correctly switched off, it is necessary that [10]:

X_{dep} =

s4SiΦn,p

qN_{D,A} > T_{Si} (3.1)

where:

• q = 1.602 × 10^{19} (C) is the elementary electric charge;

• Si= 11.7_{0} (F/cm) is the dielectric constant of the device layer;

• 0 = 8.854× 10^{−14} (F/cm) is the vacuum permittivity;

• ND,A (atoms/cm^{3}) is the device layer donor/acceptor concentration;

• qΦn,p= k_{B}T ln(N_{d,a}/n_{i}) (eV ) is the n-type/p-type Fermi potential;

• kB= 8.6173303× 10^{−5} (eV /K)is the Boltzmann constant;

• T = 293.15 (K) is the temperature;

• ni = 5.29× 10^{19}(T /300)^{2.54}e^{−6726/T} (atoms/cm^{3}) is the intrinsic carrier con-
centration [11].

That is, the maximum depletion width has to be larger than the silicon device layer thickness TSi to ensure the device full depletion. Thus the maximum depletion width (Xdep) as a function of the doping concentration (Eq.3.1) was implemented in MATLAB [12] (Appendix A.1), and the plot in Fig.3.1 was obtained.

Figure 3.1: Maximum Depletion width as a function of the doping concentration.

As can be observed in Fig.3.1, the maximum depletion width decreases with in-
creasing doping. Considering a wafer with a doping concentration of 5 × 10^{15}cm^{−3},
the corresponding maximum depletion width is 432.7nm; therefore in order to en-
sure full depletion a TSi < 432.7nm has to be obtained (e.g. 400nm). Clearly for
that doping concentration (5 × 10^{15}cm^{−3}) also a value of 10nm would guarantee full
depletion, but such thin film is more difficult to obtain from a fabrication process
point of view. In order to correctly design the silicon device layer thickness, the
doping concentrations of the wafers available for the fabrication process have to be
estimated.

### 3.1.2 Doping Concentration Estimation

Since the resistivity instead of the doping concentration is provided in Tab.2.1, it was decided to implement an iterative algorithm (Fig.3.2) in MATLAB (Appendix A.2) that on the basis of the provided resistivity can estimate the doping concentration [13]. The algorithm consists of the following steps:

1. Define a mobility value µ.

2. Compute the associated doping concentration with the given resistivity by
means of: NA= _{qρµ}^{1} .

3. Compute µ^{0} = _{1+(N/N}^{µ}^{max}^{−µ}^{min}

ref)^{α}.

4. Compute µ^{0} − µ, and verifiy if the difference is below a certain tolerance. If
it is not, define µ = µ^{0} and repeat the algorithm until the tolerance is not
satisfied.

Regarding the parameters, they were chosen according to [13]:

• Initial guess: 450 cm/V s.

• Maximum hole mobility: µmax= 495 cm/V s.

• Minimum hole mobility: µmin = 47.7 cm/V s.

• Reference concentration: Nref = 6.3× 10^{16} cm^{−3}.

• Fitting parameter: α = 0.76.

• Tolerance: tol = 0.1 cm/V s.

Start

Define µ

Compute NA and µ^{0}

|µ^{0}− µ| < tol? µ = µ^{0}

µobtained

Stop yes

no

Figure 3.2: Flow chart of the algorithm implemented in MATLAB for the mobility estimation.

The considered resistivity is 5Ωcm, since it represents the worst case analysis: lower
the resistivity, higher the doping concentration, and smaller the needed device layer
thickness (which is more difficult to obtain from a fabrication point of view). The
estimated doping concentration by means of the algorithm is 2.73 × 10^{15}cm^{−3}, while
the hole mobility is 472cm^{2}/(V s). The associated maximum depletion width is
560nm. Another possible tool is to use the graph in Fig.3.3; the value obtained with
the algorithm is coherent with the graph.

Since the device layer thickness is of critical importance for ensuring the correct operation of the transistor, it was decided to measure, with the four probe method, the real wafer resistivity and then to apply again the algorithm.

Figure 3.3: Graph of the resistivity versus impurity concentration at 300K [14].

### 3.1.3 Resistivity Measurement

The wafer resistivity can be computed with a four probe collinear measurement [15], and the basic setup is shown in Fig.3.4. A current is applied to two probes, and the voltage between the other two probes is measured. Then the wafer resistance is computed as V/I.

Figure 3.4: Schematic of a collinear four probe measurement setup [16].

Once the resistance is computed, the resistivity can be expressed as [15]:

ρ = 2πsFV

I (3.2)

where:

• s = 1mm is the spacing between two adjacent probes;

• V is the voltage measured between two probes;

• I = 1mA is the current applied to the other two probes;

• F = F1F2F3 is the correction factor;

• F1 = 2ln{[sinh(t/s)]/[sinh(t/2s)]}^{t/s} = 0.0144is the correction factor for non-conducting
bottom surface;

• t = 20µm is the wafer thickness;

• F2 = ln(2)+ln{[(D/s)^{ln(2)}^{2}+3]/[(D/s)^{2}−3]} = 0.9991 is a geometrical correction factor;

• D = 100mm is the wafer diameter;

• F3 is a boundary proximity correction factor that can be neglected [15] since the measurement is taken in the middle of wafer and the ratio of the distance between the boundary and the probes is large.

The measurements on the three wafers were carried out (measuring the voltage approximately every 60s) by means of a probe station PWS (Pacific Western System Inc) Probe II (Fig.3.5), a Keithley signal generator (for the application of constant current I = 1mA), and a Keithley multimeter (for the voltage measurement). The results are reported in Tab.3.1.

Figure 3.5: Probe station used for the resistance measurement in the clean room.

As can be observed in Tab.3.1, the resistance gradually increases with time. This can be attributed to the fact that the applied current raises the wafer temperature, thus increasing its resistivity.

Table 3.1: Wafers resistances measurement data.

Wafer Test 1 Test 2 Test 3

L 450Ω 500Ω 520Ω

C 450Ω 550Ω 650Ω

R 550Ω 650Ω 700Ω

In order to compute the resistivity through Eq.3.2, a MATALB code (Appendix A.3) was developed. The computed resistivities, together with the associated doping

concentrations computed with the algorithm in Fig.3.2 and the resulting maximum depletion widths are reported in Tab.3.2.

Table 3.2: Computed wafers resistivities, doping concentrations, and maximum de- pletion widths.

Wafer ρ N_{a} max X_{dep}

L 4.44Ωcm 3.08× 10^{15}cm^{−3} 530nm
C 4.98Ωcm 2.73× 10^{15}cm^{−3} 560nm
R 5.74Ωcm 2.35× 10^{15}cm^{−3} 600nm

Therefore the device layer thickness has to be lower of the three reported values in order to ensure full depletion; for instance the maximum depletion width of the wafer Lis 530nm. This means that a value smaller of 530nm has to be used to guarantee full depletion (e.g. 500nm). Clearly also a value of 10nm would guarantee full depletion, but such thickness is more difficult to obtain from a fabrication process point of view.

### 3.2 Source and Drain

Now that a characterization of the doping concentration level in the three wafers is provided, it is possible to start the design of the source and drain contacts, which implies decisions on the use of the material as well as on the geometrical parameters of the transistors (width and extensions).

### 3.2.1 Material Selection

When realizing a source/drain contact a metal-semiconductor junction is formed [17], and one of the most important parameter is the Schottky-barrier height, that is defined as:

Φbn = ΦM − χ (3.3)

Φ_{bp}= E_{g}− (ΦM − χ) (3.4)

for n-type and p-type semiconductor respectively, where ΦM is the metal work func- tion, χ is the silicon electron affinity, and Eg the energy band gap. Other important quantities are the semiconductor work functions defined as:

Φs,n = χ + Eg

2q − Φ^{n} (3.5)

Φ_{s,p} = χ + Eg

2q + Φ_{p} (3.6)

for n-type and p-type semiconductor respectively. They are of critical importance since on the basis of their value with respect to the metal work function the following cases can be distinguished:

• Schottky-diode contact on n-type semiconductor (Φm > Φ_{s,n});

• Schottky-diode contact on p-type semiconductor (Φm < Φ_{s,p});

• Ohmic contact on n-type semiconductor (Φm < Φ_{s,n});

• Ohmic contact on p-type semiconductor (Φm > Φ_{s,p}).

An example of energy band diagrams of a metal-semiconductor (p-type) junction
with qΦm< qΦ_{s,p} is depicted in Fig.3.6. As a forward bias is applied (Fig.3.6(c)) the
barrier height reduces, and a hole current from the semiconductor to the metal dom-
inates. By reverse biasing the junction (Fig.3.6(d)), the barrier height increases and
a very low current due to thermionic emission from the metal to the semiconductor
flows [18]. Therefore the junction is rectifying.

Figure 3.6: Energy band diagrams of a metal-semiconductor (p-type) junction with qΦm < qΦs,p. (a) Before contact. (b) In equilibrium. (c) Forward bias. (d) Reverse bias [19].

Clearly for the source/drain metallization a non-rectifying (ohmic) contact it is
needed. In order to understand the contact behavior as a function of the selected
materials, the data in Tab.3.3 were collected where a p-type doped (1e15cm^{−3})
semiconductor with qΦs,p = 4.92eV and electron affinity of 4.05eV [19] is considered.

The selected doping concentration does not coincide with the one of the three wafers but this is not critically important in this qualitative discussion because as shown in Sect.3.1.1 the Fermi potential doping concentration dependence is logarithmic.

Table 3.3: Contact behavior as a function of different materials.

Material qΦ_{M} Behavior
Al [18] 4.10eV rectifying
Ti [20] 4.33eV rectifying
W [19] 4.55eV rectifying
Cu[21] 4.65eV rectifying

The obtained results need to be carefully interpreted mainly for two reasons:

1. The metal work function is a complex parameter at which can not be associated a unique value [22]: for instance aluminum work function values from 4.06eV to 4.26eV can be found in the literature; this is due to the fact that it depends on the surface material properties (e.g. atoms configuration [23]).

2. The presented discussion is based on energy band diagram, thus it is based on a model that can not truly describe the considered physical device. For in- stance it does not consider any fabrication process consequence on the contact properties.

Therefore a design based only on work function values is not reliable, since they can not be univocally defined. In order to make ohmic a rectifying contact a typical solution [24] consists into highly dope the semiconductor near to the contact regions.

The reason can be understood by considering that when a rectifying contact is realized, a depletion region on the semiconductor side is formed [17], with expression:

Xdep =

s2_{Si}(V_{bi}− V^{a})

qN_{a} (3.7)

where Vbi is the associated built it voltage, and Va the applied voltage. If the
doping concentration is very high (> 1e19cm^{−3}) then the depletion width on the
semiconductor side is so small that tunnelling takes place, thus making the rectifying
contact behaving as an ohmic one (Fig.3.7). This is one of the reasons for which
conventional MOSFETs present highly doped pn junctions for the source and drain
contacts [25], realized through an implantation step. Another solution can be instead
to use silicidation technology, which allows through the deposition of a metal and
a successive annealing to reduce the contact resistance. But the first solution is
not compatible with the design specifications since it implies the presence of a pn
junction that by definition is absent in junctionless transistors, while the second one
it would make the process more complex and expensive, since an additional material
has to be deposited and the annealing process has to be controlled.

Figure 3.7: IV curve for two different doping concentrations [26].

Considering that the available wafers are p-doped, the simplest solution is to consider aluminum as contact material, since it is a p-type dopant for silicon [27], [28]. The resulting pp++ junction can be fabricated by deposition and successive thermal diffusion avoiding in this way implantations and thus design specifications violation.

Regarding n-type junctionless transistors, they can be fabricated by using the receipt given in [28].

### 3.2.2 Parasitic Resistance Model

In order to decide how to geometrically size the junctionless transistor under anal- ysis, it was modelled, in terms of resistances, as in Fig.3.8 where Rc is the contact resistance, Rsub the resistance associated to the region between the channel and contacts, and Rch that is the channel resistance. The latter is not considered in this section because its behavior, that depends on the applied voltage, is treated in Sect.4. The model in Fig.3.8 clearly resembles the one for conventional MOSFETs (besides the absence of the resistance associated to the extension and S/D-substrate junctions).

Figure 3.8: Schematic of the resistance modelling of the junctionless transistor.

Resistance R_{sub}

Regarding Rsub, it can be modelled as a resistive rectangular box (Fig.3.9) of length d (spacing between source/drain and gate in Fig.3.8), width W (that is the width of the transistor), thickness TSi, and resistivity ρ (measured in Sect.3.1.3). Rsub can be then expressed as:

R_{sub}= ρ d

W T_{Si} (3.8)

That is the resistance associated to the region between the S/D contacts and the channel boundary is modelled through the Pouillet’s law. Clearly this model will provide an overestimation of the parasitic resistance since the current flows along the less resistive path during operation and not in all the box.

Figure 3.9: Modelling Rsub as a rectangular box: TSi is the device layer thickness, d the spacing between the S/D and the gate, W the width of the transistor.

In order to understand the influence of the width W and the S/D-gate spacing d on Rsub, two cases are considered:

1. Fixing W to a certain value, and computing Rsub as a function of d.

2. Fixing d to a certain value, and computing Rsub as a function of W .

Case 1: fixed width W

Since the minimum photolithographic resolution of the mask aligner is 2µm, the width W is fixed to a larger value, that is 5µm. Then the resistance Rsubis computed with the implementation of a MATLAB code (Appendix A.4), and plotted as a function of d in Fig.3.10. Regarding TSi and ρ, a value of 500nm and 4.44Ωcm were respectively selected; that is the worst case analysis is considered (Wafer L in Tab.3.2), since the smallest TSi leads to the largest resistance. As can be observed, increasing the distance d, the resistance Rsub increases, and this is expected since d is in the numerator in Eq.3.8.

Figure 3.10: Case 1: Fixed W (5µm). Plot of Rsub as a function of the separation region d, which is ranging from 5µm to 10µm. Wafer under analysis is L (Tab.3.2).

Case 2: fixed separation d

The separation region d was fixed to 5µm, and the resistance Rsub was computed as a function of W , while the other parameters are the same as in Case 1. The result (Fig.3.11) is expected: as the transistor width is increased the resistance decreases.

Figure 3.11: Case 1: Fixed d (5µm). Plot of Rsub as a function of the transistor width W , which is ranging from 5µm to 10µm. Wafer under analysis is L (Tab.3.2).

On the basis of the two computations it is clear that d should have minimum value (that is its dimension coincides with the contact length), while W should be large.

The critical point is that whatever the value of d and W , the estimated resistance
R_{sub} value (∼ 1e5Ω) is unacceptable. The technological solution is to increase the
doping concentration in all the regions excepts under the channel (Fig.3.12), since
changing the doping in that region would implies a change in the needed device
layer thickness (Eq.3.1). This can be obtained through a deposition of aluminum
followed by diffusion (treated in Sect.3.2.3). On the basis of these considerations,
the structure schematic up to now is the one depicted in Fig.3.12.

Figure 3.12: Proposed structure schematic for the reduction of the high parasitic resistance Rsub (not in scale).

The structure in Fig.3.12 is clearly representing an impracticable device, since the metallization contacts are next to the metal gate, thus short circuiting the transistor.

A more correct schematic is that in Fig.3.13, where the contacts are connected to the highly doped region through a via, and an insulator separates them from the metal gate.

Figure 3.13: More realistic structure schematic for the reduction of the high parasitic resistance Rsub (not in scale).

Regarding the transistor width, it has to be considered that from a mask design point of view, the aspect ratio between the width and the length of the S/D contact, as well as of the gate, should not be too large [29]. But a well defined criterion can be selected only by considering other parameters as the contact resistance, since the latter is dependent on the transistor width.

Resistance R_{c}

The contact resistance is defined as [30]:

R_{c}= δJ
δV

_{V =0}

!−1

(3.9)
where J = JSM − J^{M S} is the total current density and V the applied voltage.

The critical problem is that accurate quantum transmission functions have to be considered in order to find a closed form of Eq.3.9[31]. In [30] the contact resistance of aluminum on silicon as a function of doping concentration for different barrier heights is reported (Fig.3.14). But is difficult to interpret the plot, because for p-type silicon only barrier heights lower than 0.5eV are reported, which are not consistent with the the theoretical barrier height that is at least 0.8eV (Eq.3.4).

Figure 3.14: Contact resistance of aluminum as a function of doping concentration for different barrier heights. Solid line (n-type silicon), dotted line (p-type silicon) [31].

Thus a different approach has to be considered; in [32] the contact resistance of alu- minum on p-type silicon is reported as a function of the silicon resistivity (Fig.3.15).

Since we are considering a p++ region under the contact area, the expected dop-

ing concentration is at least 1e20cm^{−3} [25], at which corresponds a resistivity of
approximately 0.001Ωcm [14].

Figure 3.15: Contact resistance of aluminum as a function of resistivity [32].

Therefore on the basis of the plot in Fig.3.15, a specific contact resistivity of approxi-
mately 1×10^{−7}Ωcm^{2} is expected; dividing this value by the product W Lcontact, where
the width W and the contact length Lcontact have values larger than the minimum
photolitographic resolution (W = 5µm and Lcontact= 5µm), the value of the contact
resistance is Rc ∼= 0.4Ω. For the same width and doping concentration Rsub results
to be around 2 × 10^{−5}Ωwhich is negligible with respect to Rc. This means that if a
current of 1mA flows in the transistor, a voltage drop of 0.4mV is associated to the
parasitic resistance, which is not critical for junctionless transistors whose threshold
voltage is in the 1V range; therefore a width and contact length around that value
(5µm) ideally guarantees a low parasitic resistance. It also has to be considered that
for higher doping concentration under the contact regions (1e22cm^{−3}), Rc can be
further reduced. Moreover in this analysis the contact area is considered to cover
the whole width of the transistor, while usually the latter presents an array of con-
tacts [33]. Up to now the schematic of the designed transistor is the one shown in
Fig.3.16.

Figure 3.16: Schematic of the junctionless transistor structure after resistance mod- elling (not in scale).

There are mainly two reasons for which array of contacts (Fig.3.17) are implemented in transistor fabrication process:

• Reliability, that is by placing many contacts closed to each other, microcracks in the deposited metal layer can be reduced, thus improving surface uniformity [34];

• Performance, that is by placing more than one contact is possible to reduce the contact resistance [29].

Figure 3.17: Array of contact in a MOSFET [33].

The reason for which the contact resistance can be reduced can be understood by
reasoning as follows: if, for example, for one contact window the contact resistance
is Rc,1 = 200Ω (Fig.3.18(a)), in the case in which an additional contact windows is
added to the structure (Fig.3.18(b)), then the new resistance Rc,2 is in parallel to
R_{c,1} = 200Ω, thus providing an overall contact resistance of 100Ω. Clearly also the
parasitic resistance associated to the metal has to be considered, but given the low
resistivity of aluminum, it could be neglected in this qualitative discussion.

Figure 3.18: (a)Considering only one contact window. (b) Considering two contact windows. The resistance Rm associated to the metal is not shown.

It is important to remark that the structure schematics provided in the previous sections do not represent the definitive device; for instance, it is well know that the diffusion profile is never completely flat, thus making impossible a doping profile as the one indicated in Fig.3.16, but it was decided to follow this kind of discussion flow in order to make clearer the involved problems. The values of all the geometrical parameters are reported in Sect.3.5.

### 3.2.3 Aluminum Deposition and Diffusion

Deposition

In order to have an estimation of the deposition rates of aluminum (and silicon oxide), the following process was tested in the clean room:

• deposition through sputtering of 20nm of SiO2;

• measurement of deposited SiO2 film thickness through an ellipsometer;

• deposition through sputtering of 100nm of Al;

• photoresist (PR) deposition, exposure, development;

• measurement through a profilometer of PR with respect to Al;

• Al etching, and measurement through profilometer of PR with respect to SiO2. Regarding the deposition process, it was realized with the Sputter AJA (AJA In- ternational Inc.) shown in Fig.3.19 giving as results the data provided in Tab.3.4.

Figure 3.19: Sputter AJA used for testing the aluminum deposition rate in the clean room.

Table 3.4: Process parameters for aluminum and silicon oxide deposition.

Target Thickness Pressure Power Ar Flow Dep. Rate Time

SiO2 20nm 4mtorr 100W 10sccm 0.11 30min

Al 100nm 4.1mtorr 80W 10sccm 0.2 1.38h

The deposition rates (provided by the machine itself) are quite low, thus suggesting an overall minimum deposition process time of about two hours. After the silicon oxide deposition, three measurements with an ellipsometer were taken giving as results the data collected in Tab.3.5, while an example of the ellipsometer output is given in Fig.3.20.

Figure 3.20: Third ellipsometer measurement for the silicon oxide thickness.

The measurement results are consistent with the inputs provided to the sputtering machine: the oxide thickness is around 20nm.

Table 3.5: Ellipsometer measurement data for the silicon oxide thickness.

Measurement 1 20.974nm± 0.17.7nm Measurement 2 20.970nm± 0.17.6nm Measurement 3 20.947nm± 0.16.6nm

After the silicon oxide thickness measurement, aluminum was deposited (Tab.3.4) and the following procedure was followed for the photoresist deposition:

• wafer cleaned with Isopropanol;

• bake 2min at 115°C;

• spin coating, through Spinner 2 AB Plast Spin 150, of positive PR s1813:

– time: 30s.

– speed: 3000RP M.

• bake 1min at 115°C.

and then were exposed through a Mask Aligner EVG 620, where the used mask was composed of arrays of squares, giving as result the structure in Fig.3.21.

Figure 3.21: Wafer used for testing the deposition process after exposure.

Then the exposed photoresist was developed with MF 3189, and through a Pro- filometer DEKTAK 150, three measurements in a row in the middle of the wafer were carried out giving as results the data collected in Tab.3.6.

Table 3.6: Profilometer measurement data for the estimation of the photoresist thickness in three different squares.

Measurement 1 1009.60nm Measurement 2 1005.08nm Measurement 3 1003.32nm

Therefore approximately a 1µm thick PR layer was deposited. Then the aluminum was etched with Aluminium Etch 16:1:1:2, and the structure in Fig.3.22 was ob- tained.

Figure 3.22: Wafer used for testing the deposition process after aluminum etching.

The dark areas are made of silicon oxide.

Then three measurements (along the same squares in of Tab.3.6) with the profilome- ter were taken, providing the data in Tab.3.7.

Table 3.7: Profilometer measurement data for the estimation of the aluminum thick- ness in three different squares.

Measurement 1 1122.40nm Measurement 2 1120.10nm Measurement 3 1120.16nm

It is important to remark that every measurement is done in the same associated square (that is Measurement 1 in Tab.3.6 is taken on the same square on which then Measurement 1 in Tab.3.7 is carried out) in order to have a coherent result. Sub- tracting the measurements in Tab.3.6 from the ones in Tab.3.7, gives an estimation of the deposited aluminum thickness (Tab.3.8):

Table 3.8: Profilometer measurement data for the aluminum thickness.

Al thickness 1 112.80nm Al thickness 2 115.02nm Al thickness 3 116.84nm

The thickness of the deposited aluminum layer is larger than the expected one (110nm), but this is not considered critical for the fabrication process, since the aluminum is going to be used as metallization material.

Diffusion

Once the aluminum is deposited, a diffusion process is necessary in order to make it diffuse in the silicon, thus lowering the semiconductor resistivity. The process can be modelled as a constant dose diffusion process, that is the concentration is assumed to have a gaussian distribution [35]:

N (x, t) = Q_{0}

√πDte^{−}

x 2√

Dt

^{2}

(3.10) where:

• Q0 (atoms/cm^{3}) is the deposited dose;

• D = D0e^{−}(^{Ea}kT) (cm^{2}/s) is the diffusion coefficient;

• D0 (cm^{2}/s) is an extrapolated constant;

• Ea (eV ) is the activation energy;

• k (eV/K) is the Boltzmann constant;

• T (K) is the temperature;

• t (s) is the time.

The critical point is to understand how to set the time t and temperature T in order to obtain a quasi constant distribution in the p++ regions, and how to estimate the

deposited dose Q0. The latter is a complex parameter, since its value is dependent on the crystalline structure of the deposited material, and the deposition technique.

But a simple estimation can be done in the following way:

Q0 = N_{0}ρ_{Al}T_{Al}

m_{Al} (3.11)

where:

• N0 (mol^{−1})is the number of Avogadro;

• ρAl (kg/cm^{3}) is the aluminum density;

• TAl (cm) is the thickness of the deposited layer;

• mAl (g/mol) is the aluminum molar mass.

That is, multiplying the density by the thickness of the deposited layer the surface density is obtained. So dividing the latter by the molar mass the number of moles square centimeter is obtained. Multiplying the latter by the Avogadro number pro- vides the number of atoms per square centimer. Regarding the choice of the time and the temperature, they are critically important since the dependence in Eq.3.10 is exponential. Thus a MATLAB code was implemented (Appendix A.5) to under- stand the influence of these parameters on the estimated diffusion process; a fixed temperature of 1300K (which is the maximum achievable temperature in the facil- ity) was assumed, and the concentration profile was computed for different diffusion times, giving as results the plots in Fig.3.23.

Figure 3.23: Concentration profile assuming a temperature of 1300K and a pre- deposited layer of 20nm for different diffusion times.

As expected, by increasing the time, the concentration is lowering at the surface, and the profile is less steep [35]. If instead of an aluminum deposited layer of 20nm, a thickness of 200nm is considered, the concentration profile presents higher dopants at the surface (Fig.3.24). This makes sense since in the expression provided for the dose estimation (Eq.3.11), the latter is obtained by multiplying the area density by the deposited layer thickness, so it is assumed that thicker is the deposited layer, and higher is the constant dose at the surface.

Figure 3.24: Concentration profile assuming a temperature of 1300K and a pre- deposited layer of 200nm for different diffusion times.

Since a high doping concentration implies a reduction of the parasitic resistance, a deposition of 200nm of aluminum is considered. Regarding the diffusion, a 3h process at 1300K guarantees, at least ideally, a more flat profile.

It is important to remark that the presented analysis is not considering fabrica- tion process effects such as lateral diffusion, and diffusion caused by the deposition temperature during the layer deposition step. Thus it represents a theoretical esti- mation.

### 3.3 Gate

### 3.3.1 Material Selection

The gate material is of critical important, since the flat band voltage, and con- sequently the threshold voltage, is by the definition expressed as the gate/semi- conductor work function difference [21] that for n-type and p-type transistors are respectively defined as:

V_{F B,n} = qΦ_{M} − qΦ^{s,n} = qΦ_{M} − (qχ + Eg/2 − qΦ^{n}) (3.12)

V_{F B,p} = qΦ_{M} − qΦs,p= qΦ_{M} − (qχ + Eg/2 + qΦp) (3.13)

The threshold voltage, instead, is defined as the gate voltage at which the device layer is fully depleted, where by full depletion its meant that the depletion width is equal to the device layer thickness. The expression for the depletion width of n-type and p-type semiconductors are respectively defined as:

X_{dep,n} =−_{Si}
C_{ox} +

vu
ut_{Si}

C_{ox}

2

− 2_{Si}

|q|Nd

(V_{G}− V^{F B}) (3.14)

X_{dep,p}=−_{Si}
C_{ox} +

vu
ut_{Si}

C_{ox}

2

+ 2_{Si}

|q|Na

(V_{G}− V^{F B}) (3.15)
where Cox = _{T}^{}^{ox}

ox (F/cm^{2}) is the capacitance per unit area, defined as the ratio of
the insulator dielectric constant and the insulator thickness. Regarding threshold
voltage expressions, they are obtained by imposing Xdep = T_{Si}, and solving for VG:

V_{th,n} = V_{F B} +|q|Nd

2_{Si}

"

^{2}_{Si}
C_{OX}^{2} −

t_{Si}+ _{Si}
C_{OX}

2#

(3.16)

Vth,p= VF B −|q|N^{a}
2_{Si}

"

^{2}_{Si}
C_{OX}^{2} −

tSi+ _{Si}
C_{OX}

2#

(3.17) Therefore the principle of operation of the junctionless transistor can be expressed as:

V_{G}_{ON} = V_{F B}

V_{G}_{OF F} = V_{th} = V_{F B} +^{|q|N}_{2} ^{d}

Si

"

^{2}_{Si}

C_{OX}^{2} −^{}t_{Si}+_{C}^{}^{Si}

OX

2#

(3.18) for the n-type junctionless transistor, and:

V_{G}_{ON} = V_{F B}

V_{G}_{OF F} = V_{th} = V_{F B}− ^{|q|N}_{2}_{Si}^{a}

"

^{2}_{Si}

C^{2}_{OX} −^{}t_{Si}+_{C}^{}^{Si}

OX

2#

(3.19)

for the p-type one.

The depletion width expression can be derived by applying the Poisson equation under well defined assumptions, which are discussed in details in the attached paper

"A Numerical Method to Extract the Depletion Region Width of Planar Junctionless

Transistors" (Appendix B.2) attached to this thesis. In order to understand the influence of the gate material on the flat band and threshold voltages, an analysis in term of doping concentration is carried out by considering first polylisilicon and the aluminum as gate materials.

Flat Band Voltage

A MATLAB code (Appendix A.6) was implemented in order to observe the de- pendence of the flat band voltage on the doping concentration (Eq.3.12). A first analysis was done by assuming as a gate material polysilicon, which is considered both p-doped and n-doped with work functions of 5.15eV and 4.05eV respectively [36]; that is the n-type polysilicon gate is assumed to have a work function equal to the electron affinity, while the p-type one is considered to have a work function equal to the electron affinity plus the energy band gap. Considering a n-type junc- tionless transistor, its flat band voltage behavior is depicted in Fig.3.25. As can be observed, for a p-type gate, the flat band voltage is positive, and for a difference of one order of magnitude in ND, its value is around 1V .For the n-type gate, instead, it is negative and around 0V .

Figure 3.25: Flat band voltage behavior as a function of the doping concentration for an n-type junctionless transistor.

Therefore the gate material has an influence on the polarity of the power supply, since in the case in which the flat band voltage is positive and the threhsold voltage is negative, a dual power supply is needed; if instead both the voltages are negative (or positive) then a single power supply system can be considered, thus lowering the circuit complexity. For a p-type junctionless transistor the behavior is similar, in the sense that, as can be seen in Fig.3.26, for a p-type gate the flat band voltage is positive, while for the n-type gate, instead, it is negative. But while the p- gate implies a flat band voltage value around 0V , the n-gate one implies a value around −1V . This observation is particularly important in the case in which CMOS processes are considered.

Figure 3.26: Flat band voltage behavior as a function of the doping concentration for an p-type junctionless transistor.

One of the typical problem related to the implementation of polysilicon gate in conventional MOSFET is the polydepletion effect [37]; it is remarkable that since junctionless transistors do not work in inversion, they do not suffer of such effect.

But the practical problem, from a fabrication process point of view, is that polysil-
icon is not available in the facility; moreover it would require a doping process in
order to increase its concentration to at least 1e20cm^{−3} (value for which it can be
considered to work as a metal [38]), thus increasing the fabrication process com-
plexity. In standard CMOS process a further doping implantation for doping the
polysilicon gates is not required, since they are doped during the implantation step
(the polysilicon is used as a mask for the channel). Therefore it is not convenient
to consider polysilicon as gate material. A possible solution is to use, instead, alu-
minum (qΦm= 4.1eV), which is available in the facility and does not require doping
processes. In this case the flat band voltages for the p-type junctionless transistors
under analysis are those indicated in Tab.3.9.

Table 3.9: Analytical flat band voltages considering aluminum as gate material and the measured doping concentrations of Tab.3.2.

JLT on wafer: N_{A} V_{FB}

L 3.08× 10^{15}cm^{−3} −0.8498V
C 2.73× 10^{15}cm^{−3} −0.8467V
R 2.35× 10^{15}cm^{−3} −0.8429V

Threshold Voltage

As can be seen in Eq.3.16, the threshold voltage depends also on the oxide capac- itance, which is defined as the ratio of the oxide permittivity and oxide thickness.

The latter can be sized by considering, for instance, the dielectric strength, that is the maximum electric field that the oxide can sustain before breaking. For silicon oxide this value is greater than 10MV/cm [25]. Then assuming that the junctionless transistor has a threshold voltage smaller than 5V , the power supply voltage can be assumed to have a value Vs = 5V. Considering an oxide thickness ≤ 10nm, the rigidity is then given by 6.25MV/cm which is less than 10MV/cm. Therefore in the

following analysis a value for the oxide thickness of 10nm is considered. Regarding
the permittivities of silicon and silicon oxide, they are considered to be 3.9 and 11.7
[39]. Thus a MATLAB code was implemented (Appendix A.7) in order to under-
stand the threshold voltage behavior as a function of the doping concentration; the
device layer thickness was set equal to 300nm, thus a meaningful range of doping
concentration is [1e15, 1e16]cm^{−3} since, as shown in Fig.3.1, the maximum deple-
tion width has to be larger than the silicon device layer thickness. In Fig.3.27 the
threshold voltage of a n-type junctionles transistor (with aluminum gate) is shown.

Figure 3.27: Threshold voltage behavior as a function of the doping concentration for an n-type junctionless transistor (tSi= 300nm).

As can be observed, the threshold voltage of an n-type junctionless transistor in- creases (in absolute value) with increasing doping concentration. This can be ex- plained as it follows: as the electron concentration increases, a greater voltage (in absolute value) is needed in order to repel the free electrons. A complementary ex- planation (that is reasoning in terms of holes) can be given for the threshold voltage of a p-type junctionless transistor, which is shown in Fig.3.28.

Figure 3.28: Threshold voltage behavior as a function of the doping concentration for an p-type junctionless transistor (tSi= 300nm).

Considering the three available wafers, the analytical threshold voltages can be then computed, assuming a gate oxide thickness of 10nm and a device layer thickness

T_{Si} that is 30nm less than the maximum depletion width. The analytical threshold
voltage values are reported in Tab.3.10.

Table 3.10: Analytical threshold voltage considering aluminum as gate material and and a gate oxide thickness of 10nm

JLT N_{a} Max X_{dep} T_{Si} V_{FB} V_{th}

L 3.08× 10^{15}cm^{−3} 530nm ∼ 500nm −0.8498V −0.1829V
C 2.73× 10^{15}cm^{−3} 560nm ∼ 530nm −0.8467V −0.1866V
R 2.35× 10^{15}cm^{−3} 600nm ∼ 570nm −0.8429V −0.1904V
The operating range of the designed device is therefore less than 1V ; this implies
that the device is a low voltage transistor.

Depletion Width

The depletion width analysis is not reported here, since it is treated in the attached paper to this thesis. But for a sake of completeness the curve for the JLT built on the wafer C is reported in Fig.3.29.

Figure 3.29: Analytical Depletion width of the p-type JLT built on wafer C. The threshold and flat band voltages are indicated.

As can be observed in Fig.3.29, the depletion width is equal to zero for VG = V_{F B}
(ON state), while is equal to TSi for VG= V_{th} (OFF state) as expected.